Stereolithographic Injection Molds for Direct Tooling
Suresh Jayanthi, Bronson Bokuf & Ronald McConnellDuPont Somos, Two Penn's Way, Suite 401, New Castle, DE 19720
andRobert J. Speer & Paul S. Fussell
ALCOA, 100 Technical Drive, Alcoa Technical Center, PA 15069
The use of stereolithographic core and cavity sets in low volume injection molding is
experiencing steady growth. The use of plastic instead of metal molds raises several issues in
terms of mold handling, material injection and process cycle requirements. This study focuses on
identifying and understanding these issues and optimizing them for low volume direct tooling
applications. Some experimental observations are presented using DuPont Somos epoxy
photopolymers and representative mold geometries which identify the critical mold properties
that influence mold life and the injection molded part quality.
Stereolithography (SL) is one of the rapid prototyping (RP) technologies that is a tool forreducing product development cycle times. Stereolithography creates physical models for visualinspection, form-fit studies and limited functional applications. With advances in accuracy,flatness capabilities and material properties, the push towards rapid creation of tooling using SLhas become more pronounced. Newer generations of stereolithographic photopolymers like theDuPont Somos 7100 family of materials, with their improved dimensional, mechanical andthermal properties are allowing the use of SL to directly create injection mold inserts for rapidtooling applications.
Rapid tooling approaches that use RP technologies like SL for tool fabrication are becomingan attractive alternative to traditional machining and casting techniques. The stereolithographicrapid tooling approaches essentially fall under two broad categories. The first category uses SLto make patterns and then creates conventional molds from these patterns. The second category,also called "direct tooling", uses SL to create the molds directly. The first approach is more timeconsuming because of the time required to convert a SL pattern into a conventional mold. Italways leaves room for inaccuracies being induced into the process. By eliminating the step ofmaking a mold from the SL part and using SL to directly create the mold, direct tooling holds thepromise of further reducing the time and cost needed to create low volume quantities of parts ina production material. Though some direct tooling approaches may eventually be useful for highvolume production, the limitations in speed and capability constrain their current applicability.There is no such thing as low volume tooling unless it produces quality parts. The immediateapplication for direct tooling is in the areas of prototype tooling for pre-production planning
and short run tooling for low volume production requirements. The following section will brieflyhighlight the current state of the art in low volume tooling. The remainder of this paper willprimarily focus on the stereolithographic direct tooling.
Low Volume Tooling:
As a part progresses from concept to commercial reality, it is usually necessary to buildprototypes for testing and modifications. For early functional part evaluation, the parts must bein the fmal design material. For pilot production of components, the parts must bedimensionally accurate and very similar to the production components. When manufacturingprocess development is needed, it is particularly useful to closely emulate the productionprocess itself. Of all the plastics part production techniques, injection molding dominates withmore than 92,000 machines operating in North America alone[l]. Prototype core and cavity setsplaced in a production mold base enable process simulation in making a limited number ofparts.
Tool development and fabrication using conventional techniques and materials can be timeconsuming and expensive, especially when the mold core and cavities have contours or othercomplex geometric features. In the initial stages of product development, when the final designsare still not proven, it is risky to commit to production tooling. Low volume prototype toolingis highly desirable if a limited number ofparts can be produced in a fast and economical way arerequired. Rapid tooling is best positioned to meet the needs of such low volume tooling. Byreducing the tooling costs, rapid tooling approaches enable traditional high volume processes,such as injection molding, to be competitive at lower production volumes.
Several low volume tooling options are currently used in the rapid tooling industry. Theseinclude castable steel alloy tools, milling aluminum tool inserts using a NC machine, use ofreinforced composite tools, sprayed metal tools, epoxy tooling or silicone rubber molds from SLmasters. These "soft tools" are later used in various techniques like reaction injection molding,thin walled reaction injection molding, simulated die casting, resin transfer molding and even onproduction injection molding machines. Most of these techniques enable the use of SL patternsas the starting point for rapid tooling. These approaches have been cited in the literature quiteextensively and will not be described here[3,4,5]. While they are defmitely a right step in thedirection of rapid tooling, they still entail the need for several secondary processes.
Stereolithographic Direct Tooling:
The photopolymer materials that are currently preferred for rapid tooling applications areepoxies with improved physical properties. The SL process employs layers of low molecularweight multifunctional liquid photopolymers that are locally cross linked by the exposure todirected UV light to form polymeric systems with very high molecular weight. These areessentially amorphous in nature with a high degree of cross linking of their polymer chains. Thelatest generation ofmaterials, like the DuPont Somos 7100 series, provide both improved partquality features and the needed thermal and mechanical properties. These high temperaturephotopolymers may withstand continuous exposure in air to higher temperatures withoutsignificant loss of structural integrity.
Listed below are some of the chief physical properties of stereolithographic materials thatmay have an influence on the success of SL cores and cavities in injection molding.
- Compressive Strength- Tensile Strength- Flexural Strength- Shear Strength- Impact Strength- Wear Resistance- Surface Hardness- Coefficient of thermal expansion- Thermal Conductivity- Specific Heat- Thermal Diffusivity- Heat Deflection Temperature & Glass Transition Temperature
A few other properties like the thermal fatigue characteristics and creep behavior under loadfor extended periods of time also influence the mold durability and the injection molded partquality. While the stress-strain data is normally used for metal tool design, the creep-rupturedata is more suitable for composites and plastics. Because ofviscoelasticity, the loading strengthof plastics diminishes over time. Hence, the design strength of the mold is dependent upon boththe magnitude of the applied load and the duration of its application. The strength required mustbe adequate to resist the compressive, bending and shearing stresses set up by the moldingmaterial under pressure as it moves into the mold cavity and hardens.
While many of the properties listed above are common to any tool material, heat deflectiontemperature is a characteristic unique to plastic molds. It is a measure of the temperature up towhich the material can be used without significant degradation in strength. The heat deflectiontemperature of DuPont Somos 7100 materials can be almost twice as high as most othercommercial stereolithographic materials.
Stereolithographic tools for injection molding applications are primarily used in two forms.
a) Solid core and cavity inserts that are fully formed on the SL machine.
b) Shelled core and cavity inserts which are later back filled with reinforcing, thermallyconductive materials like an aluminum filled epoxy or a low melt alloy.
Although creating the shelled core and cavity inserts reduces the SL fabrication timecompared to solid inserts, it involves subsequent steps to fill the shells with reinforcingmaterials. The thermal conductivity of solid SL molds is around 0.2 W/m-K and that of the backfilled SL molds is between 1 and 2 W/m-K. Though the gains in thermal conductivity due toback filling are not substantial compared to steel molds (typically 50 W/m-K), back filled moldsmay be effective in reducing mold cycle times. Poor thermal conductivity of the tool materialprevents the tool from allowing rapid cool down of the molding material which is needed tominimize cycle time.
There is a trend in the industry to complement the above two approaches with additionalprocessing involving treatment of the tool face with surface coatings to improve the surfacehardness and wear resistance. These treatments include electroless plating and vapor depositiontechniques. While these additional treatments may improve the tool life, they require surfacepre-treatments necessary to achieve good adhesion of the coatings to SL materials and entailadditional time and resources in the rapid tooling process.
The heat transfer rate of the SL tool inserts may also be improved with the aid of internalcooling channels. To get optimal cooling it is necessary to create conformal cooling channels.Cooling channels in close proximity to the core and cavity walls will improve heat removal andshorten cycle times. Since SL technology allows the fabrication of complex features withoutdifficulty it is possible to create cooling channels which are not necessarily circular in